Spectroscopy (AES) Scanning Auger Microscopy (SAM) scudiero/documents/571-Auger...¢ 2007....
Embed Size (px)
Transcript of Spectroscopy (AES) Scanning Auger Microscopy (SAM) scudiero/documents/571-Auger...¢ 2007....
www.wsu.edu/~scudiero Ful. 208, 5-2669
Auger Electron Auger Electron Spectroscopy (AES) Spectroscopy (AES)
Scanning Auger Scanning Auger Microscopy (SAM)Microscopy (SAM)
Louis ScudieroLouis Scudiero
High vacua at RT: 1m3 of O2 at 10-6 T weighs ~ 2 mg and the mean free path is about 51 m.
Kinetic theory: P = 1/3 Nmv2
The theory gives the frequency of collisions of gas molecules with a surface as:
N = 3/5*1022 * P * (M*T) -2
P is the partial pressure (Torr) of the gas, M the molecular weight (Sum of the atomic weighs of all the atoms in a molecule) and T gas temperature (K)
Example : O2 gas T = 20 ºC and P = 10-6 T N = 3.62 1014 molecules P = 10-9 T N = 3.62 1011 molecules
Typical clean metal surfaces have about 1015 atoms cm-2. So, if each O2 striking the surface sticks (metal/oxygen atomic ratio of 1:1).
(Briggs handbook of X-ray and UV photoelectron spectroscopy, Heyden 1977)
Time for adsorption of O2 at P = 10-6 T is 1015/3.62 1014 *2 = 1.4 s
But 24 min at 10-9 T and 4 h at 10-10 T.
NOTE Gases present in HV systems are mostly H2O vapor, CxHy, CO, H and O2. In UHV the gases are generally H and CO with some inert gases. Oxygen concentrations in UHV are generally low because reacts with CO and C on the chamber walls to produce CO and CO2
4 possible reactions:
1. Physiorption 2. Chemisorption 3. Chemisorption with reorganization and 4. Oxidation
Need for atomically clean surfaces
This concept is very important, for example if a 2 nm thick sample is covered with 1 ppm of C (10-20 monolayers), this is all that the spectroscopy would see.
Schematic of Auger Systems Typical PHI Auger instrument (600 series)
Electron emitted from the electron source are focused on the sample via electrostatic lenses. The electrons photoemitted are collected and analyzed and counted by the detector.
One or two ion guns (Ar+) are used with this technique. The Ion guns provide a way to sputter the surface of the sample and give chemical information as a function of depth (depth profiling).
First described by Pierre Auger in 1925. It was used to explain the radiationless relaxation of excited ions observed in cloud chambers. Only in 1953, J.J. Lander suggested to use it for chemical analysis. In 1968 L.A. Harris realized its importance as surface sensitive technique.
A specimen is irradiated with electrons, core electrons are ejected in the same way that an X-ray beam will cause core electrons to be ejected in XPS. Once an atom has been ionized, it must return to its ground state.
1. An X-ray photon is emitted, basis of electron probe microanalysis (EPMA).
This is carried out in many electron microscopes by either E or λ dispersive spectrometers (Geology).
2. An electron from a higher level, the L2,3 level fills the vacancy (core level), K shell vacancy.
Auger Electron Spectroscopy (AES)
Survey (Wide Scan) spectrum
CasaXPS (Washington State University, Pullman, Wa)
A rbitrary U
100 200 300 400 500 600 700 800 900 Kinetic Energy (eV)
AES is an analytical technique used to determine the elemental composition and the chemical state of the atoms in the surface of a solid material. As XPS this technique is a surface sensitive technique since the electrons have a short free path in solids. The electron escape depth (λ) is defined as the distance normal to the surface at which the probability of an electron escaping without energy loss drops to 1/e. This depends on:
1. Matrix composition (single element or composite material). 2. Energy of the Auger transition 3. Analytical geometry
For example: Auger signal from [1-exp(-d/λ)] where d is the depth and λ the IMFP. For d = λ then 63.2% of the Auger signal comes from the top 1λ, for d =2λ then 86.5% of the signal will come from the top 2λ, etc …
The energy difference between the 2 states is carried away by the ejected Auger electron. The KE of the emitted electron is characteristic of the parent
Schematic diagram of an Auger emission process in a solid. The initial state is the ground state (shown on the left), singly ionized state at the center and doubly ionized final state is shown on the right.
Auger Electron Emission Competition between X-ray fluorescence and Auger electron emission
Relative probability of Auger and x-ray fluorescence emissions. Auger and fluorescence yields as a function of atomic number. The solid lines show Auger yield; the dashed lines, fluorescence yield.
1. X-ray fluorescence (radiative decay) 2. Auger electron emission (NON-radiative decay)
Volume excited by the e- beam
Auger Electron Energy Analysis What is the Auger electron energy? Can we determine it from energy?
The energy EK - EL1 can be released as a radiative decay or non-radiative transition (Auger).
Auger kinetic energy is given by E = EK -EL1 – EL2,3 - Φ (1)
NOT SO SIMPLE
Because the transition probabilities between singly ionized and doubly ionized state of the atom (NOT GROUND STATE PROPERTIES), Ref: F.P. Larkins, Applications of Surface, Science 13, 1982, 4-34 By use of the expression (1) the Auger KE is overestimated
Example: Si and P Case 1: Si EK = 1839 eV
EL1 = 149 eV EL2,3 = 99 eV
Typical value for Φ = 4 ± 1 eV Then E = EK -EL1 – EL2 -Φ = 1587 eV This value is too high
This equation does not take into account the interaction energies between the core holes (K and L2,3) nor the intra- and extra- atomic relaxation energy which come about as a result of the additional core screening needed when there is a hole in a core level and it is achieved by an inward collapse or “relaxation” of the outer electronic orbitals towards the core.
Case 2: Z+1: then Si P For phosphorus EL1 = 189 eV
EL2,3 = 126 eV Then E = EK -EL1 – EL2 – Φ = 1552 eV
The actual energy is 1561 eV
)]1()([ 2 1)]1()([
2 1)()( 3,23,2113,2 ++−++−= ZEZEZEZEZEZE LLLLKKL
The Intra-atomic relaxation energy is the relaxation energy appropriate to an isolated atom and the extra-atomic relaxation energy is the relaxation energy from the other atoms or from the valence band due to the ionized atom in a molecule or in a solid (Coulomb and exchange integrals). A better approach is the “Z+1” approximation. The concept behind it is that after single ionization event the BE of all electrons is increased due to one less electron charge; electrostatically like Z+1 atom. Derived by Chung and Jenkins, Surface Science, 21, 253 (1970)
Lower curve: distribution of energies of secondary electrons ejected from a graphite surface by incident electrons of energy 1000 eV. The background is made of the inelastically ejected electrons and the elastic peak is shown at exactly 1000eV (often used as energy calibration).
Upper curve: differential distribution over the energy range containing the carbon KLL Auger peaks. In the differential distribution the peak ”position” is taken to be that of the high energy minimum, by convention.
Auger spectra (Cu)
a) N(E) vs E, b) dN(E)/dE vs E, c) d(E x N(E)/dE vs E , d) E x N(E) vs E
4 ways to display Auger data
Auger Si Spectrum
Oxidized Si Surface
Chemical Analysis by Auger
1st and 2nd derivative Si LVV Auger spectra of several silicides.
Scale factors for each curves were adjusted to produce similar peak intensities.
The silicide enthalpies of formation ΔHf expressed per metal atom per formula unit are also indicated.
Carbon Peaks DLC (diamond like carbon), graphite and SiC
Kinetic Energy (eV)
224 233.6 243.2 252.8 262.4 272 281.6 291.2 300.8 310.4 320
1). A distinct shoulder in the C peak of graphite was measured at KE = 280eV.
2). The Peak –Peak width is about 22 eV for graphite and DLC. It is only 9.6 eV for SiC.
3). The peak is narrower for SiC than for graphite and DLC.
Atomic Sensitivity Factors (ASF)
Voltage dependency of the Sensitivity Factors. A typical voltage used in Auger is 5kV
SAM Element Imaging
SAM element imaging provides the lateral distribution of elements in a thin film. All elements except H and He may be imaged. The “quality” and spatial resolution of SAM element images depend on the sample matrix, the quantity of the element present and the geometry of the sample. As a rule, SAM element images are of lesser quality than SEM images due to instrument and sample constraints but allows for elements analysis and element spatial distribution.
Images of a failed lead bond on a gold pad
Imaging – Spectrum a) SEM image of the interface
Ti (left)-fiber (right)
b) Boron Auger image – reaction of